# Clusters, metastability, and nucleation: Kinetics of first ... · PDF file Clusters,...

date post

24-Aug-2020Category

## Documents

view

1download

0

Embed Size (px)

### Transcript of Clusters, metastability, and nucleation: Kinetics of first ... · PDF file Clusters,...

Journal o f Statistical Physics, VoL 18, No. 1, 1978

Clusters, Metastability, and Nucleation: Kinetics of First-Order Phase Transitions M. Kalos, 1 Joel L. Lebowitz, 2 '3 '40 . Penrose, 5 and A. Sur 6

Received July 21, 1977

We describe and interpret computer simulations of the time evolution of a binary alloy on a cubic lattice, with nearest neighbor interactions favoring like pairs of atoms. Initially the atoms are arranged at random; the time evolution proceeds by random interchanges of nearest neighbor pairs, using probabilities compatible with the equilibrium Gibbs distribution at tem- perature T. For temperatures 0.59T~, 0.81To, and 0.89Tc, with density p of A atoms equal to that in the B-rich phase at coexistence, the density C~ of clusters of l A atoms approximately satisfies the following empirical formulas: C1 ~ w(1 - p)a and C~ ,.~ (1 - p)~Q,w ~ (2 ~< l ~< 10). Here w is a parameter and we define Q~ = ~K e-~K~, where the sum goes over all translationally nonequivalent /-particle clusters and E(K) is the energy of formation of the cluster K. For l > 10, Qz is not known exactly; so we use an extrapolation formula Q~ ~ AwZ~l -~ e x p ( - b P ) , where w~ is the value of w at coexistence. The same formula (with w > w~) also fits the observed values of C~ (for small values of l) at densities greater than the coexistence density (for T = 0.59T~): When the supersaturation is small, the simula- tions show apparently metastable states, a theoretical estimate of whose lifetime is compatible with the observations. For higher supersaturation the system is observed to undergo a slow process of segregation into two coexisting phases (and w therefore changes slowly with time). These results may be interpreted as a more quantitative formulation (and confirmation) of ideas used in standard nucleation theory. No evidence for a " sp inoda l " transition is found.

KEY W O R D S : Cluster destruction; metastable states; nucleation kinetics; computer simulation; lattice gas; binary alloy.

Supported by AEOSR Grant No. 73-2430D and by E R D A Contract No. EY-76-C-02- 3077*000.

1 Courant Institute of Mathematical Sciences, New York University, New York, New York.

2 John Guggenheim Fellow on sabbatical leave from Belfer Graduate School of Science, Yeshiva University, New York, New York.

3 Service de Physique Theorique, CEN, Saclay, France. 4 Permanent address: Depar tment of Mathematics, Rutgers University, New Brunswick,

New Jersey. 5 The Open University, Milton Keynes, England. 6 Belfer Graduate School of Science, Yeshiva University, New York, New York.

39

oo22-4715/78/OlOO-OO395o5.oo/o �9 1978 Plenum Publishing Corporation

40 M. Kalos, Joel L. Lebowitz, O. Penrose, and A. Sur

1. I N T R O D U C T I O N

The object of this paper is to summarize and interpret the results of some computer simulations which demonstrate, among other things, the possibility of metastable states in a binary alloy (and in the corresponding lattice gas).

In earlier papers of this series ~1-4~ we described the results of computer simulations of the time evolution of such an alloy following quenching from a high temperature (where the equilibrium state is spatially uniform) to a low temperature for which the equilibrium state has comparable amounts of two different phases. In following the system's evolution (at the lower tem- perature) from the initial "macroscopically" uniform state to a state in which there are distinct regions containing A-rich and B-rich phases, our main tool was the Fourier transform of the pair correlation function. In the present paper we summarize and interpret the results of simulations where the true equilibrium state after quenching still has two phases, but only a small amount of one of them. In the language of the density-temperature diagram, we are still quenching to points inside the two-phase region, but they are now close to the coexistence curve. This part of the diagram is called the nucleation region. Our tool for investigating the time evolution is now the analysis of clusters of the minority atoms.

We find that at points close to the coexistence curve (i.e., small super- saturation in the lattice gas language) the system can stay for very long times in a metastable state of uniform macroscopic density. As the supersaturation is increased, the rate at which nucleation and segregation of the new phase take place increases in an apparently continuous fashion until we find our- selves in the rapidly varying regime studied earlier. No sharp "spinodal transition" from metastable to unstable states was observed, although the probability of nucleating a critical cluster changes rapidly with the degree of supersaturation. This fits in with our earlier findings that the Cahn- Hilliard linearized theory, ~ which among other things also predicts such a transition, does not yield a good description of the computer simulations. Similar conclusions have also been drawn by other authors ~6,r~ on the basis of both theory and experiment.

The simulations were done on the CDC 6600 computer at the ERDA Mathematics and Computer Laboratory at New York University. The program simulates a simple cubic lattice of N sites (where N = 125 • 103 or 27 x 103) with periodic boundary conditions, each site of the lattice having two states, "occupied" and "unoccupied" (in the interpretation appropriate for alloys, an "occupied" site holds an A atom and an "unoccupied" site holds a B atom). At the initial time, a specified number pN of randomly chosen sites are put in the "occupied" state and the rest in the "unoccupied" state. The program chooses a pair of neighboring sites at random, then

Clusters, Metastability, and Nucleation 41

exchanges their occupation states (i.e., the atoms on them) with a probability given by

[exp(-f l AE)]/[1 + exp(-/3 AE)] (1)

where/3 = 1 /kT is a constant and AE is the increase in energy caused by the interchange. The energy is defined as

E = - V Z n~nj, n~ = 0,1 (2) t,1

where V is a constant, n~ is the occupation number of the ith site, and the sum goes over all nearest neighbor pairs of sites. The transition probability (1) satisfies the detailed balancing condition for equilibrium at temperature 1//cB/3.

As the simulation proceeds, the computer periodically records informa- tion about the current configuration. In particular, it calculates the sizes of all the clusters (maximal connected sets of occupied sites) in the configura- tion. This information about clusters yields, at low densities, a description of the configurations which provides a convenient way to understand what is going on, and makes possible some quantitative comparisons between theory and simulation.

2. Q U A L I T A T I V E D E S C R I P T I O N OF T H E D A T A

Most of the simulation runs reported on here were done at a temperature T such that/3 V = 1.5; that is, T = 0.59Tc, where Tc is the critical temperature, which is known very accurately from series expansions/a~ The lowest density studied was p = 0.0146, which, according to the Pad6 approximant formula, ~a~ is the saturated vapor density at this temperature. The simulation runs at this density show, as we would expect, a distribution of cluster sizes which varies rapidly at first, since the initial random state corresponds to equilibrium at infinite temperature rather than at 0.59T~, but soon settles down (after about 50 attempted exchanges per site) to an equilibrium in which no cluster of more than 11 particles was ever observed.

At the next density, 0.02, the behavior is qualitatively very similar, but with somewhat more clusters of each size than at density 0.0146. The largest cluster observed among the configurations recorded contained 26 particles, and clusters of this size usually lasted only a short time. There was no observable tendency for the cluster distribution to change with time (apart from fluctuations) and since this state has a higher density than that of the standard " v a p o r " phase, we interpret it as a metastable state.

At the next density studied, p -- 0.035, the distribution of small clusters appears to reach equilibrium in about the same time as before, 50-100

42 M. Kalos, Joel L. Lebowitz, O. Penrose, and A. Sur

attempted exchanges per site; but it takes longer (about 400 attempted exchanges per site) for the number of clusters in the size range 30-50 to build up. By the end of the run (about 450 attempted exchanges per site) the number of clusters in this size range appeared to be fairly steady, but the runs were not long enough to decide definitely whether the state at this density could be regarded as metastable.

At densities 0.05 and 0.06, a new pattern of behavior is beginning to show itself. Once again a fairly stable distribution of cluster sizes is established after about 50-100 attempted exchanges per site, but now this distribution is itself slowly changing with time: The number of large clusters (larger than, say, 50) is seen to build up slowly with time, as is the number of particles in such clusters, while the number of particles in small clusters (ten particles or less) can be seen, despite the fluctuations, to be decreasing steadily on the average. Thus, in the p = 0.05 case the total number of particles in clusters of ten or fewer particles decreases from about 5400 (i.e., 0.043 per site) after 100 attempted exchanges per site to about 4800 (i.e., 0.035 per site) after 500 attempted exchanges per site; and in the p = 0.06 case the same effect was e